Gate Tunable Relativistic Mass and Berry’s phase in Topological Insulator Nanoribbon Field Effect Devices Luis A. Jauregui1,2, Michael T. Pettes3*, Leonid P. Rokhinson1,2,4, Li Shi3,5 & Yong P. Chen1,2,4

Received 23 December 2014 Accepted 7 January 2015 Published 13 February 2015

Correspondence and requests for materials should be addressed to Y.P.C. (yongchen@ purdue.edu)

* Current address: Department of Mechanical Engineering, University of Connecticut, Storrs, CT 06269.

1

Birck Nanotechnology Center, Purdue University, West Lafayette, IN 47907, 2School of Electrical and Computer Engineering, Purdue University, West Lafayette, IN 47907, 3Department of Mechanical Engineering, University of Texas at Austin, Austin, TX 78712, 4Department of Physics and Astronomy, Purdue University, West Lafayette, IN 47907, 5Materials Science and Engineering Program, University of Texas at Austin, Austin, TX 78712.

Transport due to spin-helical massless Dirac fermion surface state is of paramount importance to realize various new physical phenomena in topological insulators, ranging from quantum anomalous Hall effect to Majorana fermions. However, one of the most important hallmarks of topological surface states, the Dirac linear band dispersion, has been difficult to reveal directly in transport measurements. Here we report experiments on Bi2Te3 nanoribbon ambipolar field effect devices on high-k SrTiO3 substrates, where we achieve a gate-tuned bulk metal-insulator transition and the topological transport regime with substantial surface state conduction. In this regime, we report two unambiguous transport evidences for gate-tunable Dirac fermions through p Berry’s phase in Shubnikov-de Haas oscillations and effective mass proportional to the Fermi momentum, indicating linear energy-momentum dispersion. We also measure a gate-tunable weak anti-localization (WAL) with 2 coherent conduction channels (indicating 2 decoupled surfaces) near the charge neutrality point, and a transition to weak localization (indicating a collapse of the Berry’s phase) when the Fermi energy approaches the bulk conduction band. The gate-tunable Dirac fermion topological surface states pave the way towards a variety of topological electronic devices.

T

he extraordinary electronic properties of topological insulators1–3 (TIs) make them a unique class of materials relevant for applications such as low power electronic devices, spintronics1 and fault-tolerant quantum computation4,5. TIs feature topologically non-trivial surface states, where carriers are massless relativistic particles with linear energy-momentum band dispersion and with spins locked perpendicular to their momentum2,3. Existence of such helical Dirac fermion surface states have been experimentally confirmed by angle-resolved photoemission spectroscopy (ARPES)6,7 and scanning-tunneling microscopy8. Transport measurements in bulk crystals of TI (such as Bi2Te3)9 have met more challenges to probe the surface states, because of the non-insulating bulk conduction. In order to reduce the bulk contribution and enhance the surface contribution in TI transport, a number of efforts have been made by growing bulk single-crystals with fine-tuned composition10–13, adding compensating dopants14,15, growing ultrathin films and nanostructures such as nanowires16,17 or nanoribbons (NRs)11,18, and using electrical gating19–21 to tune the Fermi energy (EF). Nanostructures, with a high surface-to-volume ratio, have been shown to enhance the surface conduction contribution. However, in previous reports, unambiguous measurements of the topological surface states (e.g p-Berry’s phase and Dirac fermion dispersion) remain challenging. In this work, we combine nanostructures with ultrahigh-k gate dielectric by placing Bi2Te3 NRs on SrTiO3 (STO) substrates22,23. We realize the topological transport regime where bulk is insulating and surface substantially contributes to the conduction, and report clear evidence of the Dirac fermion nature of the gate-tunable topological surface states, directly revealing the characteristic linear energymomentum dispersion via density-dependent effective mass measurements. The excellent gate tunability of EF (from surface states to bulk conduction band) has also enabled us to observe a predicted transition from the usual weak anti-localization (WAL) behavior to weak localization (WL), reflecting a change in the pseudospin texture and Berry’s phase of the quantum coherent charge carriers24,25. The Bi2Te3 NRs were synthesized by catalyst-free vapor solid method, following an approach similar to that of Kong et al.26 for thin films. NRs are grown out of the plane of the substrate and they are individually transferred to other substrates or support for further studies, using an electrochemically sharpened tungsten probe and an optical microscope. We have used transmission electron microscopy (TEM) to determine the structural

SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

1

www.nature.com/scientificreports characteristics of the Bi2Te3 NRs. Low-magnification TEM reveals a typical width of ,100–230 nm and a length exceeding 10 mm (Fig. 1a). High-resolution TEM confirms the single-crystallinity, with ˚ (Fig. 1b, marked with arrows) along the an atomic spacing of 2.2 A ½1120 direction, similar to previously grown single-crystal Bi2Te3 NRs21. The Fourier transform (FFT) of the high-resolution TEM image reveals a high-quality single-crystalline structure with hexagonal symmetry (inset of Fig. 1b). We have also performed Raman spectroscopy with a 532 nm excitation laser on Bi2Te3 NRs (placed on SiO2/Si substrates). Figure 1c shows a representative spectrum. We observe three Raman peaks at 62 cm21, 104 cm21 and 137 cm21, in excellent agreement with the Raman optical phonon modes (A11g , Eg2 and A21g ) previously measured in bulk crystals27 and exfoliated thin flakes28,29 of Bi2Te3, further confirming the good crystalline quality of our NRs. Fig. 1d shows the atomic force microscope (AFM) image of a typical NR with thickness , 30 nm and width ,130 nm. Most of the electronic transport data presented below (unless otherwise noted) are measured from this representative Bi2Te3 NR, which is transferred onto a 500-mm-thick STO substrate (with very high relative dielectric permittivity k at low temperatures30) and fabricated into a back gated field effect device (device #1). Similar results have also been obtained in several other devices measured. Temperature dependence and field effect. Effective gate control of topological surface states is highly desired for investigations of novel quantum transport and many device applications of TIs4,21. The optical image of device #1 and a schematic of its cross section are shown in the lower and upper insets of Fig. 2a, respectively. Figure 2a also shows the ambipolar field effect measured in the NR at 2K, where the decreasing backgate voltage (Vg) tunes the carriers from n-type to p-type, with the resistance (R) peaking at the charge neutrality point (VCNP , 217 V). We note that VCNP should be

above the Dirac point, which is shown to be buried inside the BVB from previous ARPES measurements on bulk Bi2Te3. The typical gated R modulation ratio is , 3–10 in our field effect devices. For Vg 5 0 V, the temperature (T) dependence of the resistance (R(T)) of the Bi2Te3 NR device (Fig. 2b) shows a metallic behavior (R decreases with decreasing T), as previously observed in highly doped samples with bulk-dominated conduction9. However, for Vg 5 26.5 V and 215 V, we observe an insulating behavior (R increases with decreasing T, due to bulk carrier freeze-out) for 10 K , T , 30 K with R saturating at a Vg-dependent value (Rsat) for T , 10 K. This Rsat corresponds to EF inside the bulk bandgap and the low-T metallic conduction of topological surface states (TSS, see band schematic in the inset of Fig. 2b). For Vg 5 222 V and 230 V (Vg , VCNP), in addition to the insulating behavior and low-T Rsat, we observe R(T) peaks at T , 10 K. This peak resistance is similar to the peak resistance measured at Vg 5 VCNP from the field effect (Fig. 2a, see also Fig. S1a, note the peak value can vary slightly after thermal cyclings), and is attributed to the strong enhancement of k of STO30 at low T, such that EF is lowered to cross CNP and further into the bulk valence band (VB) as T decreases (see also Fig. S1b, and its inset demonstrating T-dependence of VCNP). Our data shows that at low T, we can use Vg to tune EF (schematically represented with dashed lines in the inset of Fig. 2b) all the way from the conduction band (CB) to the TSS then to the VB. The measured R(T) suggests that bulk carriers in our Bi2Te3 NRs can be suppressed with Vg to realize a bulk insulating regime where surface can contribute dominantly to the conduction, and this is further corroborated with magnetotransport measurements presented later. A bulk metallic-to-insulator transition has also been observed in our Bi2Te3 NRs fabricated on SiO2/Si (eg., Fig. S2, device #4), while we have focused more on devices with STO backgate as they are found to generally give stronger gate tuning for ambipolar field effect31.

Figure 1 | Material characterizations of Bi2Te3 nanoribbons. (a) Transmission electron microscope (TEM) image of a 150 nm wide Bi2Te3 nanoribbon (NR). NRs grow along the ½1120 direction. (b) High-resolution TEM image, with the corresponding Fourier transform depicted in the inset. The obtained lattice spacing of 2.2 A˚ is consistent with the lattice spacing of f1120g planes16,26. (c) A representative Raman spectrum (measured with a 532 nm laser) showing characteristic Raman peaks (labeled) similar to those observed in bulk Bi2Te3 (inset depicts corresponding phonon modes27,28) (d) Atomic force microscope (AFM) image of a 130 nm wide Bi2Te3 NR (device #1 before fabrication) on a SrTiO3 (STO) substrate. A thickness of 30 nm is extracted from the AFM line profile (inset, measured along the blue line in the AFM image). SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

2

www.nature.com/scientificreports

Figure 2 | Gate-tuned bulk metal-insulator transition and ambipolar field effect. (a) Ambipolar field effect (4-terminals resistance R vs. Vg), measured at T 5 2 K. The upper (lower) inset depicts a schematic cross section (optical image, top view, with the inner electrodes used to measure the voltage separated by 850 nm) of the fabricated Bi2Te3 NR device #1 on a 500 mm-thick STO substrate. (b) Temperature (plotted in log scale) dependence of R of device #1 measured at five gate voltages (Vg). Inset: schematic of the band diagram of Bi2Te3. The horizontal dashed lines depict 3 representative locations of the Fermi energy (EF), intercepting with the bulk conduction band (CB), topological surface states (TSS) and bulk valence band (VB), respectively. Note the Dirac point (DP) is buried inside the VB, thus only n-type TSS carriers are accessible inside the bulk bandgap.

Aharonov-Bohm Oscillations. When an external magnetic field (B) is applied along the length of the NR, the low-T magnetoconductance (G(B)) displays periodic oscillations (Fig. 3a) in B, commonly known as Aharonov-Bohm (A-B) oscillations (or ‘‘h/e oscillations’’) with a characteristic period (DB 5 Wo/A), where Wo 5 h/e is the flux quantum, A is the NR cross-sectional area (width3height), h is Planck’s constant and e is the electron charge. In contrast, for bulk carriers there are impurity-dependent loops with no well-defined cross sectional area, resulting in universal conductance fluctuations (UCF), with non-periodic B-field dependence. A-B oscillations were previously observed in Bi2Te3 and Bi2Se3 NRs21,32. In order to probe the surface states, we measure G vs. parallel B-field from device #1 (Fig. 3a) at four representative Vg’s. For Vg 5 210, 211 and 213 V, periodic oscillations are clearly observed in Fig. 3a with DB , 1T (vertical dashed lines). This DB agrees well with Wo/A 5 1.06 T for our device, therefore these oscillations are the A-B oscillations, with G maxima at integer multiples of Wo (top axes). However for Vg 5

4 V (EF inside CB), the oscillations become non-periodical and they are attributed to UCFs due to bulk carriers. The FFT of G (with a polynomial background subtracted) vs. 1/B for Vg 5 210 V and T 5 0.3 K is depicted in the left inset of Fig. 3a. We observe a dominant peak (,0.98 T21), which is the period of the A-B oscillations. This period corresponds to an area A , 4000 nm2, again in good agreement with the AFM-measured cross-sectional area of the NR (,3900 nm2) of device#1 (Fig. 1d). The right inset of Fig. 3a displays the T-dependence of the amplitude (from FFT) of the A-B oscillations for Vg 5 -10 V, where a T21/2 dependence is observed (other Vg’s show similar behavior). Such a T21/2 dependence is consistent with previous work in TI NRs21,32 and has also been observed in diffusive metallic33 and semiconducting rings34. We have also observed AB oscillations in two other devices (#2-3) with different cross sectional areas (A 5 19800 and 3600 nm2 respectively). The measured period DB vs. Vg are depicted in Fig. 3b, along with the data from device#1. We observe that DB is independent of Vg, but instead is

Figure 3 | Aharonov-Bohm oscillations of the surface carriers. (a) Magnetoconductance (G) vs. magnetic field (B, with the corresponding magnetic flux W plotted on the top axis) applied parallel to the NR length (device #1) at 4 different Vg’s (curves vertically offset for clarity, except for Vg 5 -13 V) measured at T 5 0.3 K. Left inset: FFT of G (Vg 5 -10 V) vs. 1/B, after a background subtraction in G. Right inset: temperature dependence of the FFT amplitude for the h/e oscillations at Vg 5 -10 V; a fitting with a T-0.5 dependence is plotted as a solid line. (b) Period (DB) of oscillations vs. Vg for three devices with different cross section areas (A 5 3900, 19800 and 3600 nm2 for devices 1, 2 and 3 respectively). The inset depicts magnetic flux (DB . A, in units of h/e) for these 3 devices (including all data points measured at different Vg’s shown in the main panel). SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

3

www.nature.com/scientificreports controlled by A such that the product DB.A (magnet flux corresponding to DB) is , h/e (flux quantum) for all 3 devices (inset of Fig. 3b), confirming these oscillations are A-B oscillations of surface carriers. Shubnikov-de Haas oscillations. Figure 4a shows the magneto resistance (R(B)) vs. B-field (perpendicular to the NR surface and the substrate), measured for device #1 at T 5 1.5 K and Vg 5 28 V, where small oscillations are observed. The top inset of Fig. 4a displays DR (R(B) with a smooth polynomial background subtracted) at high B-field vs. 1/B, where periodical oscillations in 1/B are clearly observed. These oscillations are Shubnikov-de Haas (SdH) oscillations due to the formation of Landau levels (LL) in high magnetic fields. We take the FFT of DR (bottom inset of Fig. 4a) to find the frequency of oscillations (BF) , 55.4 T. The Fermi momentum (kF) and carrier density (nSdH) can be obtained from 1=BF ~4p e=(hk2F ) and nSdH ~gk2F =4p respectively, where g 5 1 is the degeneracy for spin polarized surface state (we attribute the SdH as coming from one surface, most likely the back-gated bottom surface, whereas another surface has much lower mobility and less conduction9,10,35). For the data shown in Fig. 4a, we obtain nSdH 5 1.27 ˚ 21. We extract the phase of the SdH 3 1012 cm22 and kF 5 0.028 A oscillations (which will correspond to a Berry’s phase) following the standard procedure by plotting the integer Landau level index (n) vs. 1/B (Landau level fan diagram), as shown in Fig. 4b for several Vg’s. An integer n is defined at DR minima (open markers) and n 1 0.5 is

defined at DR maxima (solid markers). The assignment of integer n’s to DR minima, similar to the convention used in previous SdH studies in TINRs, is appropriate given the relatively large surface contribution to the conductance in our ultrathin NR samples (see a good discussion in ref. 36, also see Fig. S5). It is clearly seen that n fits (shown as lines) linearly with 1/B (n 5 BF/B 1 b), the slope (BF) varies with Vg and we extrapolate b , 0.5 for all Vg’s (right inset of Fig. 4b, noting SdH oscillations were only observable in the range of Vg from 28 to 213 V with n-type TSS carriers). This b , 0.5 is further confirmed by a direct fitting (an example shown as the black solid line in Fig. 4a top inset) of the SdH oscillations to the low-T theoretical expression DR* exp {p =mSdH surface B cosð2p ðBF =Bz0:5zbÞÞ (yielding

also BF and SdH mobility mSdH surface consistent with values from FFT/LL analysis above and SdH analysis discussed below). We have also plotted BF ( / nSdH) vs. Vg in the left inset of Fig. 4b, where the expected linear dependence from the effect of gating is observed. The LL indices for both Schrodinger and Dirac fermions can be linearly fitted to 1/B. However, it is well known that b 5 0 for Schrodinger fermions and b 5 1/2 for massless Dirac fermions, with the Berry’s phase given by 2p b (Refs. 13, 37-39 ). Such a prominent 1/2-shifted SdH effect provides a strong transport evidence of the spin-helical topological surface state Dirac fermions with the nontrivial Berry’s phase p. The amplitude of the SdH oscillations decreases with increasing T (while at each Vg, we found that nSdH does not change substantially

Figure 4 | Shubnikov-de Haas (SdH) oscillations of surface state Dirac fermions showing linear E-k dispersion. (a) Representative magnetoresistance (R vs. B) with B applied perpendicular to the NR plane, measured at Vg 5 -8 V and T 5 1.5 K for device #1. Top inset: DR (R with a background substracted) vs. 1/B (red, with a fit shown as black curve and FFT shown as bottom inset). (b) 1/B vs. LL index (fan diagram) at different Vg’s. Right inset: b (intercept of LL index for 1/B R0 as extracted from the fan diagram) vs. Vg. Left inset: SdH oscillation frequency (BF, left axis, inverse slope of 1/B vs. LL index) and density nSdH (right axis) vs. Vg (solid line is a linear fit) (c) Extracted effective mass (m*) vs. carrier density (nSdH 5 eBF/h), where m* is pﬃﬃﬃﬃﬃﬃﬃﬃﬃ extracted by equation (3) from the temperature dependence of the SdH oscillations. The dashed line is a fit to nSdH p behavior. The ﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃﬃ ﬃ inset shows DR/R vs. T, for LL index 5 5. (d) Effective mass m* (left axis) as well as Fermi energy (EF 5 m*ÆvFæ2) vs. Fermi momentum (kF ~ 4p eBF =h), where ÆvFæ is the average (and mostly constant) Fermi velocity (nF ~ hkF =m*) over the nSdH range measured (inset). Black dashed line represents a calculated linear dependence using ÆvFæ as Fermi velocity. SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

4

www.nature.com/scientificreports with T in the range of temperature where SdH is observed). By fitting the T-dependence of the SdH oscillation amplitudes to the LifshitzKosevich formula (Methods, and an example in Fig. 4c inset) we extract the cyclotron frequency (vC 5 eB/m*) at the B-field position of a given Rxx minimum, corresponding to the Nth LL. At each Vg (with corresponding nSdH), the effective mass (m*) is obtained from the linear fit of vC vs. B-field. The extracted pﬃﬃﬃﬃﬃﬃﬃﬃﬃ m* vs. nSdH (Fig. 4c) is not constant, rather proportional to nSdH , a distinct character for massless Dirac fermions previously demonstrated in graphene38,39. hkF =m*) is nearly independent The calculated Fermi velocity (nF ~ of nSdH (inset of Fig. 4d), with a mean value (ÆvFæ , 5 3 105 m/s), in reasonable agreement with vF measured by ARPES in Bi2Te3 bulk crystals6 (vF 5 4.1 3 105 m/s). Figure 4d shows the corresponding Fermi energy (EF 5 m*ÆvFæ2) as well as the m* vs. kF, where a linear dependence of EF (and m*) with kF is demonstrated (dashed line represents a calculated linear dependence EF ~m n2F ~ hnF kF using vF 5 ÆvFæ as constant Fermi velocity). pﬃﬃﬃﬃﬃﬃﬃﬃﬃ The density-independent vF, gate-tunable m* , nSdH and therefore the linear band dispersion (EF vs. kF) obtained in our experiments are in good agreement with the linear energy dispersion measured by ARPES in bulk Bi2Te36,7, and are clear evidences that carriers in Bi2Te3 NRs behave as massless Dirac fermions in electronic transport. We have extracted the (high-magnetic-field) quantum lifetime (tq) of surface carriers for each Vg (Fig. S3 shows 2 examples) from the slope of ln (DRB sinh (2p 2 kB T= hvC )) vs. 1/B (so called ‘‘Dingle analysis’’, see Methods and Supplemental Materials). We also calculated the corresponding high-field quantum mean free path ( q 5 vFtq), SdH etq SdH SdH mobility mSdH surface ~ , and SdH conductivity ssurface ~enSdh msurface m (See Fig. S4) of the surface carriers that give SdH oscillations at T 5 1.5 K. Since it is expected that tq,ttr, where ttr is the transport lifetime (contributed mainly by large-angle scattering rather than by all scatterings as in tq)40 of surface state carriers at B 5 0 T, the calculated mSdH surface

and sSdH surface provide lower bounds for the (zero-field) transport mobility surface. We (msurface) and conductivity (ssurface) of the corresponding . have plotted the (dimensionless) ratio sSdH surface stotal vs. the gate voltage

in Fig. S5, where stotal 5 (L/W)/R is the total (2D sheet) conductivity of the NR (measured at zero-magnetic-field, with L, W and R being the length, width and 4-terminals resistance of the TI NR, respectively; noting all conductivities in this paper are 2D sheet conductivities). For the reasons discussed above (due to tq,ttr) and the fact that the contribution from only one surface.(that gives SdH oscillations) is SdH included in sSdH surface , this ratio (ssurface stotal ) underestimates the actual

surface contribution to the total conductance. The large value of sSdH surface =stotal (reaching ,0.5 at Vg , -8 V) is notable, confirming that the surface can make substantial or even dominant contribution (manifested in the residual saturating metallic resistance seen in the R vs T in Fig. 2b) to the total conductance at low T (where bulk is insulating at this Vg). The reduction of sSdH surface =stotal for decreasing Vg (towards VCNP) might be related to the shape of the bandstructure of Bi2Te3 near the Dirac point (DP), which is buried inside the bulk VB (Fig. 2b inset). Weak antilocalization and localization. Weak antilocalization (WAL) appears as a negative magnetoconductivity (Ds(B) 5 s(B) – s(B 5 0 T)) with a sharp cusp centered at zero B-field. It is commonly observed in TIs due to the spin-momentum locking resulting from strong spin-orbit coupling. The p-Berry’s phase carried by the topological surface states of TIs leads to destructive interference between time-reversed paths, enhancing s(B 5 0T). The WAL cusp can be destroyed by applying a B-field that breaks the time reversal symmetry and p-Berry’s phase41. We use the simplified Hikami-Larkin-Nagaoka formula41,42 to fit Ds(B): ! " !# e2 h 1 h z { ln Y DsHLN (B)~a0 ð1Þ ph 4eBL2w0 2 4eBL2w0

Figure 5 | Gate-tuned weak antilocalization (WAL) and transition to weak localization (WL). (a) Magnetoresistance (R vs. B, with B applied perpendicular to the NR plane) at 5 different Vg’s at T 5 1.5 K for device #1. (b) Magnetoconductivity (Ds(B), where Ds(B) 5 s(B) - s(B 5 0 T)), normalized by e2/h. Solid lines depict fitting to HLN equation (see text). (c) Weak antilocalization (WAL) prefactor a0 (left axis) and phase coherence length LW0 (right axis), both extracted using the HLN fit, as functions of Vg (for negative Vg). (d) Weak localization (WL) prefactor a1 (left axis) and phase coherence lengths (right axis) for WAL and WL contributions (solid lines are guides to the eye), extracted from the two-component HLN fit, with fixed a0 5 -0.5, for Vg . 2 V. SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

5

www.nature.com/scientificreports where Y is the digamma function, LQ0 is the phase coherence length, and a0 is a prefactor. Each coherent channel that carries a p-Berry’s phase should give a0 5 -1/2. In contrast, if the Berry’s phase is absent, the destructive interference mentioned above would become constructive, resulting in weak localization (WL). The WL appears as a positive magnetoconductivity that can be similarly fitted to Eq. (1) with a positive a0. Figure 5a shows the magnetoresistance R(B) measured at 1.5 K at five different Vg’s. By increasing Vg from 218 V to 114 V, we observe that R(B) transitions from exhibiting a dip (indicating negative Ds(B), and WAL) to a peak (indicating positive Ds(B), and WL) near zero B field. Figure 5b displays the anti-symmetrized Ds(B) (extracted from the R(B)) vs. B-field at these Vg’s, where the gate induced transition from negative to positive Ds(B) (WAL to WL) is clearly observed. Also, we note that the amplitude of the WAL or WL cusp depends on Vg. We first focus on the gate-tunable WAL for Vg , 0 V. Using equation 1, we fit Ds (B) (for B , 2 T) at different Vg’s and extract the gatedependent a0 and LQ0 (Fig. 5c). We observe a0 peaks , 21 for Vg , 218 V (,VCNP) and approaches 20.5 for either Vg . 212 V (EF approaching the CB) or Vg , 230 V (EF near the VB). The parameter a0 is related to the number of coherent conduction channels A 5 2ja0j. The transition from a 5 20.5 (A 5 1, away from CNP) to a 5 21 (A 5 2, near CNP) tuned by Vg reflects the transition of the system from a single coherent channel (with bulk and TSS strongly coupled together) to two decoupled coherent channels surrounding the two surfaces (as bulk conduction is suppressed by the gate22,25,42,43). Also, LQ0 displays a minimum of , 62 nm for Vg , VCNP. For Vg $ 2 V, Ds(B) transitions into positive and weak localization (WL) behavior, although a small WAL (negative Ds(B)) can still be observable at very low B fields (B , 0.2 T, as shown in Fig. 5b), reflecting a competition (mixed contributions) between WAL and WL. We perform a twocomponent fit for Ds(B) using equation 2, derived by Lu-Shi-Shen (LSS)44, to extract the WAL (a0, LQ0) and WL (a1, LQ1) contributions, ! " !# X ai e2 h 1 h Ds(B)~ z { ln Y : ð2Þ 4eBL2wi 2 4eBL2wi ph i~0,1 In order to obtain unique fitting results for the WAL and WL parameters (using equation 2), we fix the WAL prefactor a0 5 20.5 (a reasonable choice given Fig. 5c shows a0 saturates at ,20.5 for Vg .212 V). We observe (Fig. 5d) that as Vg increases from 2 V to 14 V, both the WL prefactor a1 (,1) and WAL phase coherence length LW0 (, 120 nm) remain relatively constant, while the WL phase coherence length LW1 moderately increases from 46 to 76 nm. Transitions from WAL to WL in TIs have previously been observed in magnetically doped TIs45 and extremely thin TI flakes (4–5 nm thick)46,47, and are attributed in both cases to gap opening in the surface states (i.e., DP destroyed)44,48. It has been theoretically predicted that TI can also display a competition between WAL and WL, without involving surface gap opening and destroying the DP, if EF is close to the transition region between TSS and the bulk bands (CB or VB)24,25. It has been pointed out that as EF moves from the TSS to near the bottom of CB, the Berry’s phase decreases from of p to 0 (due to change in the pseudospin texture, where the bulk bandgap can act as a fictitious Zeeman field perpendicular to the spin-orbit field), giving rise to a WAL to WL transition24,25. Observing such WAL to WL transition as predicted24,25 is another piece of evidence that we are actually observing topological surface states transport.

Conclusions In conclusion, we have achieved ambipolar field effect on single crystal Bi2Te3 NRs using STO as substrate and backgate dielectric. We are able to use the gate to tune the electronic transport from being dominated by the metallic bulk to a bulk-insulating regime such that surface state contributes mostly to the conduction at low SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

temperatures. We observed gate-controlled A-B oscillations of surface carriers. We have also measured gate-controlled SdH oscillations with an extracted p-Berry’s phase, m* proportional to square root of carrier density, and nearly constant vF, providing direct evidence of the Dirac fermion nature (linear EF vs. kF) of the topological surface states. Also, a gate-tunable WAL is observed and the extracted number of coherent conduction channels is found to peak around 2 (corresponding to 2 decoupled channels surrounding 2 surfaces) for Vg , VCNP. Finally, we observe a competition between WAL and WL for Vg . 0 V, consistent with a predicted collapse of Berry’s phase and change of pseudospin texture as EF approaches the CB. The gate-tunable topological surface states found in our samples pave the way towards topologically protected nanoelectronic and spintronic devices and possible applications in topological quantum computing with Majorana fermions. During the revision of the previous version of our manuscript, we became aware of another experiment on Bi2Te3 that also reported the observation of linear dispersion and relativistic mass in SdH oscillations49.

Methods Nanoribbons synthesis and transfer. Bulk Bi2Te3 (99.999%, Alfa Aesar) was placed in the center of a single-zone furnace (TF55035A-1, LindburgH BlueMH) and SiO2 covered Si substrates were placed downstream. The temperature was slowly ramped (1–2uC/min) to ,480uC under flowing Ar (,75 cm3/min, 99.999% purity) and pressure was maintained in the range of 20–70 Torr for the duration of the synthesis. Growth times were on the order of 1–3 hours. Transmission electron microscopy (TEM). Transmission electron microscopy (200 kV, JEM-2010F, JEOL Ltd.) analysis of several NRs showed growth along the ½1120 direction and energy dispersive X-ray spectroscopy indicated excess tellurium (66 6 2 at.% Te). The tips of the NRs were observed to be catalyst free with f1010g facets. Raman Spectroscopy. Raman spectroscopy was performed using a Horiba Jobin Yvon Xplora confocal Raman microscope. The wavelength of the excitation laser was 532 nm and the power of the laser incident on the sample was kept below 200 mW to avoid sample burning. The laser spot size was , 0.6 mm with a 100X objective lens (numerical aperture 5 0.90). The spectral resolution was 1.0 cm21 (using a grating with 2400 grooves/mm) and each spectrum was an average of 3 acquisitions (5 seconds of accumulation time per acquisition). Atomic Force Microscopy (AFM). The width and thickness of the samples was measured by a NT-MDT NTEGRA Prima multifunctional atomic force microscope in tapping mode configuration. In order to avoid any damage or NRs displacement, we use a small cantilever driving amplitude and set point amplitude corresponding to 75% of the freely resonant magnitude. The silicon probes used are ACTA series from AppNANO, with a nominal 40 N/m spring constant, cantilever length of 125 mm and 6 nm radius of curvature. Device fabrication and electronic transport measurements. Our STO substrates are single side polished (100) from Shinkosha Ltd. The electrical contacts (Cr/Au, 5 nm/ 70 nm, e-beam evaporated) to Bi2Te3 NRs were patterned by e-beam lithography. Right before the metal deposition, a short etch (20 sec.) in a dilute solution of sulfuric acid (H2SO45H2O, 1510) is performed to remove native oxide from the surface. After the metal evaporation, the device is mounted and wirebonded to a ceramic chip carrier. Cr/ Au (10/70 nm) is deposited on the backside of STO (backgate electrode). All the electrical measurements are performed in a top loading Helium-3 system (Heliox TL system, Oxford Instruments). The resistances were measured by 4-terminals method and using low frequency lock-in detection (PAR124A), with a driving current of ,1 mA. Temperature dependence of the Shubnikov de Haas oscillations and effective mass calculation. We fit the T-dependence of SdH oscillation amplitude (DR) to the Lifshitz-Kosevich theory50: DR(T,B)!

2p 2 kB T=hvC e{p =vC tq sinh½2p 2 kB T=hvC

ð3Þ

Where vC and tq are the fitting parameters and B is the magnetic field position of the Nth minimum in DR; kB is the Boltzmann’s constant; vC 5 eB/m* is the cyclotron frequency (and hvC is the cyclotron energy gap for the Nth LL); m* is the effective mass of the carriers and tq is the quantum lifetime. The vC is calculated from the fitting of the relative amplitude DR/R(B 5 0T) as a function of T using equation (3) (inset of Fig. 4c) for different LLs. The m* is extracted from the slope of vC vs. B for a given Vg. 1. Moore, J. E. The birth of topological insulators. Nature 464, 194 (2010). 2. Hasan, M. Z. & Kane, C. L. Colloquium: Topological insulators. Reviews of Modern Physics 82, 3045 (2010).

6

www.nature.com/scientificreports 3. Qi, X.-L. & Zhang, S.-C. Topological insulators and superconductors. Reviews of Modern Physics 83, 1057 (2011). 4. Cook, A. & Franz, M. Majorana Fermions in a Topological Insulator Nanowire Proximity-Coupled to an S-Wave Superconductor. Phys. Rev. B 84, 201105 (2011). 5. Fu, L. & Kane, C. Superconducting proximity effect and majorana fermions at the surface of a topological insulator. Phys. Rev. Lett. 100, 96407 (2008). 6. Chen, Y. L. et al. Experimental Realization of a Three-Dimensional Topological Insulator, Bi2Te3. Science 325, 178 (2009). 7. Hsieh, D. et al. A tunable topological insulator in the spin helical Dirac transport regime. Nature 460, 1101 (2009). 8. Zhang, T. et al. Experimental Demonstration of Topological Surface States Protected by Time-Reversal Symmetry. Phys. Rev. Lett. 103, 266803 (2009). 9. Qu, D.-X., Hor, Y., Xiong, J., Cava, R. & Ong, N. Quantum oscillations and hall anomaly of surface states in the topological insulator Bi2Te3. Science 329, 821 (2010). 10. Jun, X. et al. Quantum oscillations in a topological insulator Bi2Te2Se with large bulk resistivity (6Vcm). Physica E: Low-dimensional Systems and Nanostructures 44, 917 (2012). 11. Kong, D. et al. Ambipolar field effect in the ternary topological insulator (BixSb(1-x))2Te3 by composition tuning. Nat. Nanotechnol. 6, 705 (2011). 12. Ren, Z., Taskin, A., Sasaki, S., Segawa, K. & Ando, Y. Large bulk resistivity and surface quantum oscillations in the topological insulator Bi2Te2Se. Phys. Rev. B 82, 241306 (2010). 13. Taskin, A., Ren, Z., Sasaki, S., Segawa, K. & Ando, Y. Observation of dirac holes and electrons in a topological insulator. Phys. Rev. Lett. 107, 016801 (2011). 14. Analytis, J. G. et al. Two-dimensional surface state in the quantum limit of a topological insulator. Nature Physics 6, 960 (2010). 15. Wang, Z. et al. Tuning carrier type and density in Bi2Se3 by Ca-doping. Appl. Phys. Lett. 97, 042112 (2010). 16. Kong, D. S. et al. Topological Insulator Nanowires and Nanoribbons. Nano Lett. 10, 329 (2010). 17. Tian, M. L. et al. Dual evidence of surface Dirac states in thin cylindrical topological insulator Bi2Te3 nanowires. Sci Rep 3, 7 (2013). 18. Hong, S., Cha, J., Kong, D. & Cui, Y. Ultra-low carrier concentration and surfacedominant transport in antimony-doped Bi2Se3 topological insulator nanoribbons. Nat. Commun. 3, 757 (2012). 19. Steinberg, H., Gardner, D., Lee, Y. & Jarillo-Herrero, P. Surface State Transport and Ambipolar Electric Field Effect in Bi2Se3 Nanodevices. Nano Lett. 10, 5032 (2010). 20. Yuan, H. et al. Liquid-gated ambipolar transport in ultrathin films of a topological insulator Bi2Te3. Nano Lett. 11, 2601 (2011). 21. Xiu, F. X. et al. Manipulating surface states in topological insulator nanoribbons. Nat. Nanotechnol. 6, 216 (2011). 22. Chen, J. et al. Tunable Surface Conductivity in Bi2Se3 Revealed in Diffusive Electron Transport. Phys. Rev. B 83, 241304 (2011). 23. Chen, J. et al. Gate-Voltage Control of Chemical Potential and Weak Antilocalization in Bi2Se3. Phys. Rev. Lett. 105, 176602 (2010). 24. Lu, H. Z. & Shen, S. Q. Weak localization of bulk channels in topological insulator thin films. Phys. Rev. B 84, 125138 (2011). 25. Garate, I. & Glazman, L. Weak localization and antilocalization in topological insulator thin films with coherent bulk-surface coupling. Phys. Rev. B 86, 035422 (2012). 26. Kong, D. et al. Few-layer nanoplates of Bi2Se3 and Bi2Te3 with highly tunable chemical potential. Nano Lett. 10, 2245 (2010). 27. Richter, W., Kohler, H. & Becker, C. R. Raman and far-infrared investigation of phonons in rhombohedral V2-VI3 compounds - Bi2Te3, Bi2Se3, Sb2Te3 and Bi2(Te1-XSeX)3 (0 , x,1), (Bi1-YSbY)2Te3 (0 , y,1). Physica Status Solidi B-Basic Research 84, 619 (1977). 28. Shahil, K., Hossain, M., Teweldebrhan, D. & Balandin, A. Crystal symmetry breaking in few-quintuple Bi2Te3 films: Applications in nanometrology of topological insulators. Appl. Phys. Lett. 96, 153103 (2010). 29. Teweldebrhan, D., Goyal, V. & Balandin, A. A. Exfoliation and Characterization of Bismuth Telluride Atomic Quintuples and Quasi-Two-Dimensional Crystals. Nano Lett. 10, 1209 (2010). 30. Couto, N., Sace´pe´, B. & Morpurgo, A. Transport through graphene on SrTiO3. Phys. Rev. Lett. 107, 225501 (2011). 31. Tian, J. F. et al. Quantum and Classical Magnetoresistance in Ambipolar Topological Insulator Transistors with Gate-tunable Bulk and Surface Conduction. Sci Rep 4, 4859 (2014). 32. Peng, H. L. et al. Aharonov-Bohm interference in topological insulator nanoribbons. Nat. Mater. 9, 225 (2010). 33. Washburn, S., Umbach, C. P., Laibowitz, R. B. & Webb, R. A. TemperatureDependence of the Normal-Metal Aharonov-Bohm Effect. Phys. Rev. B 32, 4789 (1985).

SCIENTIFIC REPORTS | 5 : 8452 | DOI: 10.1038/srep08452

34. Hansen, A. E., Kristensen, A., Pedersen, S., Sorensen, C. B. & Lindelof, P. E. Mesoscopic decoherence in Aharonov-Bohm rings. Phys. Rev. B 64, 045327 (2001). 35. Xiong, J. et al. High-field Shubnikov-de Haas oscillations in the topological insulator Bi2Te2Se. Phys. Rev. B 86, 045314 (2012). 36. Veldhorst, M. et al. Magnetotransport and induced superconductivity in Bi based three-dimensional topological insulators. physica status solidi (RRL) - Rapid Research Letters 7, 26 (2013). 37. Sacepe, B. et al. Gate-tuned normal and superconducting transport at the surface of a topological insulator. Nat. Commun. 2, 575 (2011). 38. Zhang, Y., Tan, Y.-W., Stormer, H. & Kim, P. Experimental observation of the quantum Hall effect and Berry’s phase in graphene. Nature 438, 201 (2005). 39. Novoselov, K. et al. Two-dimensional gas of massless Dirac fermions in graphene. Nature 438, 197 (2005). 40. Davies, J. H. The Physics of Low-dimensional Semiconductors: An Introduction. (Cambridge University Press, 1998). 41. Hikami, S., Larkin, A. I. & Nagaoka, Y. Spin-Orbit Interaction and Magnetoresistance in the Two Dimensional Random System. Progress of Theoretical Physics 63, 707 (1980). 42. Steinberg, H., Laloe¨, J., Fatemi, V., Moodera, J. & Jarillo-Herrero, P. Electrically tunable surface-to-bulk coherent coupling in topological insulator thin films. Phys. Rev. B, 233101 (2011). 43. Checkelsky, J. G., Hor, Y. S., Cava, R. J. & Ong, N. P. Bulk Band Gap and Surface State Conduction Observed in Voltage-Tuned Crystals of the Topological Insulator Bi2Se3. Phys. Rev. Lett. 106, 196801 (2011). 44. Lu, H. Z., Shi, J. R. & Shen, S. Q. Competition between Weak Localization and Antilocalization in Topological Surface States. Phys. Rev. Lett. 107, 076801 (2011). 45. Liu, M. H. et al. Crossover between Weak Antilocalization and Weak Localization in a Magnetically Doped Topological Insulator. Phys. Rev. Lett. 108, 036805 (2012). 46. Zhang, L. et al. High quality ultrathin Bi2Se3 films on CaF2 and CaF2/Si by molecular beam epitaxy with a radio frequency cracker cell. Appl. Phys. Lett. 101, 153105 (2012). 47. Lang, M. R. et al. Competing Weak Localization and Weak Antilocalization in Ultrathin Topological Insulators. Nano Lett. 13, 48 (2013). 48. Qi, X. L., Hughes, T. L. & Zhang, S. C. Topological Field Theory of Time-Reversal Invariant Insulators. Phys. Rev. B 78, 195424 (2008). 49. Gooth, J., Hamdou, B., Dorn, A., Zierold, R. & Nielsch, K. Resolving the Dirac cone on the surface of Bi2Te3 topological insulator nanowires by field-effect measurements. Appl. Phys. Lett. 104, 243115 (2014). 50. Schoenberg, D. Magnetic Oscillations in Metals. (Cambridge University Press, 1984).

Acknowledgments The TI material synthesis, characterization and magneto-transport studies are supported by DARPA MESO program (Grant N66001-11-1-4107). The FET fabrication and characterizations are supported by Intel Corporation. L. A. J. acknowledges support by the Intel PhD fellowship and the Purdue Center for Topological Materials. L.P.R. acknowledges support by NSF grant DMR-1307247. We also acknowledge helpful input from Jaehyun Kim.

Author contributions L.A.J. designed and fabricated the devices and carried out the measurements. M.T.P. and L.S. synthesized the Bi2Te3 nanoribbons and performed structural analysis. L.P.R. and Y.P.C. contributed to the measurements and analysis. Y.P.C. supervised the research. L.A.J. and Y.P.C. wrote the paper with contributions from all other co-authors.

Additional information Supplementary information accompanies this paper at http://www.nature.com/ scientificreports Competing financial interests: The authors declare no competing financial interests. How to cite this article: Jauregui, L.A., Pettes, M.T., Rokhinson, L.P., Shi, L. & Chen, Y.P. Gate Tunable Relativistic Mass and Berry’s phase in Topological Insulator Nanoribbon Field Effect Devices. Sci. Rep. 5, 8452; DOI:10.1038/srep08452 (2015). This work is licensed under a Creative Commons Attribution 4.0 International License. The images or other third party material in this article are included in the article’s Creative Commons license, unless indicated otherwise in the credit line; if the material is not included under the Creative Commons license, users will need to obtain permission from the license holder in order to reproduce the material. To view a copy of this license, visit http://creativecommons.org/licenses/by/4.0/

7